Statistical optimization of guest uptake in crystalline sponges: grading structural outcomes.
Carroll, Robert C.; Coles, Simon J.; IUCrJ 11 (2024) –; doi:10.1107/S2052252524004871

data_1571868
_publ_section_title
;
 Statistical optimization of guest uptake in crystalline sponges: grading
 structural outcomes.
;
_journal_coeditor_code           LT5068
_journal_issue                   4
_journal_name_full               IUCrJ
_journal_paper_doi               10.1107/S2052252524004871
_journal_volume                  11
_journal_year                    2024
_chemical_formula_moiety         'C72 H48 I12 N24 Zn6, 0.7(C15 H16 O3)'
_chemical_formula_sum            'C82.5 H59.2 I12 N24 O2.1 Zn6'
_chemical_formula_weight         3335.39
_chemical_name_systematic
; (2',6'-dimethoxy-[1,1'-biphenyl]-2-yl)methanol
 (absorbed in crystalline sponge)
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           13
_space_group_name_Hall           '-P 2yac'
_space_group_name_H-M_alt        'P 1 2/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_audit_creation_date             2024-01-30
_audit_creation_method
;
Olex2 1.5-alpha
(compiled 2023.11.24 svn.r209d9fb2 for OlexSys, GUI svn.r6869)
;
_cell_angle_alpha                90
_cell_angle_beta                 102.214(2)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   31.6622(7)
_cell_length_b                   15.0003(2)
_cell_length_c                   34.4418(8)
_cell_measurement_reflns_used    15885
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      74.0400
_cell_measurement_theta_min      2.8320
_cell_volume                     15987.6(6)
_computing_cell_refinement       'CrysAlisPro 1.171.41.89a (Rigaku OD, 2020)'
_computing_data_collection       'CrysAlisPro 1.171.41.89a (Rigaku OD, 2020)'
_computing_data_reduction        'CrysAlisPro 1.171.41.89a (Rigaku OD, 2020)'
_computing_molecular_graphics    'Olex2 1.5-alpha (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5-alpha (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2016/6 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      100(2)
_diffrn_detector                 'hybrid pixel array detector'
_diffrn_detector_area_resol_mean 10
_diffrn_detector_dtime           0.000
_diffrn_detector_type            'Rigaku, HyPix 6000HE'
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  t~exp~   \w     \q     \k     \f   Frames
--------------------------------------------------------------------------
  1  \w   -151.00 -90.00   0.50    2.00    -- -103.00 -18.00 150.00  122
  2  \w   -174.00-139.00   0.50    2.00    -- -103.00 -30.00-120.00   70
  3  \w   -174.00-148.00   0.50    2.00    -- -103.00-125.00-120.00   52
  4  \w   -103.00 -30.00   0.50    2.00    -- -103.00  77.00-120.00  146
  5  \w    -60.00 -33.00   0.50    2.00    -- -103.00  61.00  30.00   54
  6  \w   -103.00 -31.00   0.50    2.00    -- -103.00  77.00 150.00  144
  7  \w   -103.00 -76.00   0.50    2.00    -- -103.00  77.00  60.00   54
  8  \w    -70.00 -32.00   0.50    2.00    -- -103.00  77.00  60.00   76
  9  \w    -69.00 -43.00   0.50    2.00    -- -103.00  61.00 -30.00   52
 10  \w   -135.00 -77.00   0.50    2.00    -- -103.00-125.00-120.00  116
 11  \w    -65.00 -39.00   0.50    2.00    -- -103.00  61.00 -60.00   52
 12  \w    -69.00 -34.00   0.50    2.00    -- -103.00  61.00 150.00   70
 13  \w    -84.00 -38.00   0.50    2.00    -- -103.00  77.00 -90.00   92
 14  \w    -60.00 -33.00   0.50    2.00    -- -103.00  61.00  90.00   54
 15  \w     91.00 154.00   0.50    2.00    --  101.75  18.00 -41.00  126
 16  \w     65.00 106.00   0.50    2.00    --  101.75 -94.00  30.00   82
 17  \w    106.00 175.00   0.50    2.00    --  101.75  15.00-120.00  138
 18  \w    -22.00   3.00   0.50    0.40    --  -46.48  18.00 -41.00   50
 19  \w   -112.00 -36.00   0.50    0.40    --  -46.48 -18.00 150.00  152
 20  \w    -24.00   1.00   0.50    0.40    --   46.48 -18.00 150.00   50
 21  \w     38.00 120.00   0.50    0.40    --   46.48  18.00 -41.00  164
 22  \w     -4.00  23.00   0.50    0.40    --  -46.48  19.00  90.00   54
 23  \w    -27.00  43.00   0.50    0.40    --   46.48 -37.00   0.00  140
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_details
'Rigaku Oxford Difffraction, UG2 \k goniometer'
_diffrn_measurement_device_type
; Rigaku 007HF equipped with Varimax confocal mirrors and a UG2 goniometer 
and HyPix 6000HE detector
;
_diffrn_measurement_method       'profile data from \w-scans'
_diffrn_measurement_specimen_support 'MiTeGen loops'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      -0.0326249000
_diffrn_orient_matrix_UB_12      0.0142615000
_diffrn_orient_matrix_UB_13      0.0268843000
_diffrn_orient_matrix_UB_21      0.0375165000
_diffrn_orient_matrix_UB_22      0.0202085000
_diffrn_orient_matrix_UB_23      0.0353379000
_diffrn_orient_matrix_UB_31      -0.0029208000
_diffrn_orient_matrix_UB_32      0.0996587000
_diffrn_orient_matrix_UB_33      -0.0110301000
_diffrn_radiation_collimation    0.3
_diffrn_radiation_monochromator  'Varimax focusing mirrors'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Cu K\a'
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0732
_diffrn_reflns_av_unetI/netI     0.0493
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       38
_diffrn_reflns_limit_h_min       -37
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       41
_diffrn_reflns_limit_l_min       -40
_diffrn_reflns_number            103356
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        67.684
_diffrn_reflns_theta_max         68.248
_diffrn_reflns_theta_min         1.723
_diffrn_source                   'Rotating anode'
_diffrn_source_current           30.0
_diffrn_source_power             1.2
_diffrn_source_target            Cu
_diffrn_source_type              'Rigaku 007 HF'
_diffrn_source_voltage           40.0
_exptl_absorpt_coefficient_mu    19.475
_exptl_absorpt_correction_T_max  0.309
_exptl_absorpt_correction_T_min  0.107
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.41.89a (Rigaku Oxford Diffraction, 2020)
Analytical numeric absorption correction using a multifaceted crystal
model based on expressions derived by R.C. Clark & J.S. Reid.
(Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'light yellow'
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    yellow
_exptl_crystal_density_diffrn    1.386
_exptl_crystal_description       block
_exptl_crystal_F_000             6220
_exptl_crystal_size_max          0.22
_exptl_crystal_size_mid          0.14
_exptl_crystal_size_min          0.11
_refine_diff_density_max         1.581
_refine_diff_density_min         -1.525
_refine_diff_density_rms         0.278
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.039
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1363
_refine_ls_number_reflns         29162
_refine_ls_number_restraints     1310
_refine_ls_restrained_S_all      1.020
_refine_ls_R_factor_all          0.1587
_refine_ls_R_factor_gt           0.1433
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.2455P)^2^+405.6700P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.4434
_refine_ls_wR_factor_ref         0.4536
_reflns_Friedel_coverage         0.000
_reflns_number_gt                21798
_reflns_number_total             29162
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            lt5068.cif
_cod_data_source_block           50_5_96b
_cod_original_formula_sum        'C82.50 H59.20 I12 N24 O2.10 Zn6'
_cod_database_code               1571868
_shelx_shelxl_version_number     2016/6
_chemical_oxdiff_formula         '(Zn3 I6 N12 H24 C36) (C15 H16 O3)2 (C6 H12)2'
_chemical_oxdiff_usercomment     JP-9300-04
_shelx_estimated_absorpt_t_max   0.223
_shelx_estimated_absorpt_t_min   0.100
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All C(H,H) groups
 At 1.5 times of:
  All C(H,H,H) groups, All O(H) groups
2. Restrained distances
 C8A-C7A = C9A-C8A = C9A-C10A = C11A-C10A = C12A-C11A = C7A-C12A
 1.39 with sigma of 0.02
 C5A-C13A
 1.51 with sigma of 0.02
 C7A-C9A = C8A-C10A = C9A-C11A = C10A-C12A = C11A-C7A = C12A-C8A
 2.4 with sigma of 0.04
 C5A-O1A
 2.4 with sigma of 0.02
 C12A-C15A
 2.4 with sigma of 0.02
 O2A-C14A \\sim O1A-C13A \\sim O3A-C15A
 with sigma of 0.02
 O2A-C8A \\sim O3A-C12A
 with sigma of 0.02
 I310-Zn35 \\sim I410-Zn45
 with sigma of 0.02
 I309-Zn35 \\sim I409-Zn45
 with sigma of 0.02
 Zn35-N318 \\sim Zn45-N318
 with sigma of 0.02
 Zn35-N319 \\sim Zn45-N319
 with sigma of 0.02
 I310-I309 \\sim I410-I409
 with sigma of 0.04
 I310-N318 \\sim I410-N318
 with sigma of 0.04
 I310-N319 \\sim I410-N319
 with sigma of 0.04
 I309-N318 \\sim I409-N318
 with sigma of 0.04
 I309-N319 \\sim I409-N319
 with sigma of 0.04
 I404-Zn42 \\sim I304-Zn32
 with sigma of 0.02
 I403-Zn42 \\sim I303-Zn32
 with sigma of 0.02
 Zn42-N305 \\sim Zn32-N305
 with sigma of 0.02
 I404-I403 \\sim I304-I303
 with sigma of 0.04
 I404-N305 \\sim I304-N305
 with sigma of 0.04
 I403-N305 \\sim I303-N305
 with sigma of 0.04
 I302-Zn31 \\sim I402-Zn41
 with sigma of 0.02
 I301-Zn31 \\sim I401-Zn41
 with sigma of 0.02
 Zn31-N301 \\sim Zn41-N301
 with sigma of 0.02
 I302-I301 \\sim I402-I401
 with sigma of 0.04
 I302-N301 \\sim I402-N301
 with sigma of 0.04
 I301-N301 \\sim I401-N301
 with sigma of 0.04
 I309-Zn35 \\sim I2-Zn55
 with sigma of 0.02
 I310-Zn35 \\sim I1-Zn55
 with sigma of 0.02
 I307-Zn34 \\sim I407-Zn44
 with sigma of 0.02
 I308-Zn34 \\sim I408-Zn44
 with sigma of 0.02
 Zn34-N312 \\sim Zn44-N312
 with sigma of 0.02
 Zn34-N313 \\sim Zn44-N313
 with sigma of 0.02
 I307-I308 \\sim I407-I408
 with sigma of 0.04
 I307-N312 \\sim I407-N312
 with sigma of 0.04
 I307-N313 \\sim I407-N313
 with sigma of 0.04
 I308-N312 \\sim I408-N312
 with sigma of 0.04
 I308-N313 \\sim I408-N313
 with sigma of 0.04
3. Uiso/Uaniso restraints and constraints
C7A \\sim C3A \\sim C4A \\sim C2A \\sim C5A \\sim C1A \\sim C8A \\sim C12A
\\sim C13A \\sim C6A \\sim O2A \\sim C9A \\sim O3A \\sim C11A \\sim O1A \\sim
C14A \\sim C10A \\sim C15A: within 2A with sigma of 0.04 and sigma for terminal
atoms of 0.08 within 2A
4. Rigid body (RIGU) restrains
 C336, I306, Zn33, I305, N306, N307, C318, C314, Zn43, C319, C323, C317, H318,
 H314, C315, I406, I405, H319, C320, H323, C322, H317, C316, H315, H320, C321,
 H322, C308, C324, N302, N304, N308, N309, C306, C307, C326, C325, C303, N303,
 C309, N310, C334, C327, C302, C304, C310, C313, C333, C335, C328, C331, H302,
 C301, H304, C305, C311, H310, H313, C312, H333, C332, H335, H328, C329, C330,
 H331, N301, H301, H305, N305, H311, H312, H332, N312, H336, N311, H329, H330,
 Zn31, Zn41, Zn51, Zn32, Zn42, Zn34, Zn44, I302, I301, I401, I402, I502, I501,
 I304, I303, I404, I403, I307, I308, N313, I407, I408, C337, C341, H337, C338,
 H341, C340, C339, H338, H340, C342, N314, N315, C344, C343, N316, C352, C345,
 C353, C351, C349, C346, H353, C354, C350, H351, H349, C348, C347, H346, N318,
 H354, H350, H348, N317, H347, Zn35, Zn45, Zn55, I310, I309, N319, I410, I409,
 I1, I2, C355, C359, C356, H355, C358, H359, H356, C357, H358, C360, N320, N321,
  C362, C361, N322, C370, C363, C371, C369, C367, C364, C372, H371, C368, H369,
 C366, H367, C365, H364, H372, N324, H368, H366, N323, H365, Zn36, Zn46, I311,
 I312, I412, I411
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
5. Others
 Sof(I406)=Sof(Zn43)=Sof(I405)=1-FVAR(1)
 Sof(I306)=Sof(I305)=Sof(Zn33)=FVAR(1)
 Sof(I412)=Sof(Zn46)=Sof(I411)=1-FVAR(2)
 Sof(I311)=Sof(I312)=Sof(Zn36)=FVAR(2)
 Sof(Zn32)=Sof(I304)=Sof(I303)=1-FVAR(3)
 Sof(I404)=Sof(I403)=Sof(Zn42)=FVAR(3)
 Sof(I407)=Sof(Zn44)=Sof(I408)=1-FVAR(4)
 Sof(I307)=Sof(I308)=Sof(Zn34)=FVAR(4)
 Fixed Sof: I310(0.54342) I309(0.54342) I302(0.56585) I301(0.56585)
 Zn35(0.54342) Zn31(0.56585) Zn45(0.43399) I410(0.43399) I409(0.43399)
 I1(0.02259) I2(0.02259) Zn55(0.02259) C3A(0.70013) H3A(0.70013) C2A(0.70013)
 H2A(0.70013) C1A(0.70013) H1A(0.70013) C6A(0.70013) H6A(0.70013) C5A(0.70013)
 C4A(0.70013) O2A(0.70013) O3A(0.70013) C7A(0.70013) C8A(0.70013) O1A(0.70013)
 H1AA(0.70013) C13A(0.70013) H13A(0.70013) H13B(0.70013) C11A(0.70013)
 H11A(0.70013) C9A(0.70013) H9A(0.70013) C10A(0.70013) H10A(0.70013)
 C12A(0.70013) C14A(0.70013) H14A(0.70013) H14B(0.70013) H14C(0.70013)
 C15A(0.70013) H15A(0.70013) H15B(0.70013) H15C(0.70013) I401(0.40333)
 Zn41(0.40333) I402(0.40333) I502(0.03082) I501(0.03082) Zn51(0.03082)
 Fixed Uiso: I1(0.08) I2(0.08) Zn55(0.08) I502(0.08) I501(0.08) Zn51(0.08)
6.a Secondary CH2 refined with riding coordinates:
 C13A(H13A,H13B)
6.b Aromatic/amide H refined with riding coordinates:
 C349(H349), C366(H366), C317(H317), C367(H367), C318(H318), C302(H302),
 C356(H356), C304(H304), C348(H348), C305(H305), C372(H372), C355(H355),
 C371(H371), C358(H358), C313(H313), C320(H320), C359(H359), C333(H333),
 C368(H368), C369(H369), C335(H335), C319(H319), C328(H328), C365(H365),
 C314(H314), C323(H323), C337(H337), C364(H364), C315(H315), C332(H332),
 C322(H322), C336(H336), C330(H330), C311(H311), C312(H312), C301(H301),
 C353(H353), C331(H331), C310(H310), C347(H347), C354(H354), C338(H338),
 C346(H346), C341(H341), C329(H329), C350(H350), C340(H340), C351(H351),
 C3A(H3A), C2A(H2A), C1A(H1A), C6A(H6A), C11A(H11A), C9A(H9A), C10A(H10A)
6.c Fitted hexagon refined as free rotating group:
 C3A(C2A,C1A,C6A,C5A,C4A)
6.d Tetrahedral OH refined with riding coordinates:
 O1A(H1AA)
6.e Idealised Me refined as rotating group:
 C14A(H14A,H14B,H14C), C15A(H15A,H15B,H15C)
;
_shelx_res_checksum              75573
_shelx_hkl_checksum              4480
_olex2_date_sample_data_collection 2022-06-13
_olex2_date_sample_submission    2022-06-13
_olex2_submission_original_sample_id 50_5_96b
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
- Detector area scaling
- B-factor correction
;
_oxdiff_exptl_absorpt_empirical_full_max 3.152
_oxdiff_exptl_absorpt_empirical_full_min 0.409